LMucko/crystallography-open-database huggingface dataset:
Order and miscibility in the otavite - magnesite solid solution Sample: X_Mg = .2, synthesized at 600 C, 1 GPa, 3 h
Bromiley, F. A.; Boffa Ballaran, T.; Langenhorst, F.; Seifert, F.; American Mineralogist 92 (2007) 829–836; doi:10.2138/am.2007.2315

data_9010205
_publ_section_title
;
 Order and miscibility in the otavite - magnesite solid solution
 Sample: X_Mg = .2, synthesized at 600 C, 1 GPa, 3 h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              829
_journal_page_last               836
_journal_paper_doi               10.2138/am.2007.2315
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Synthetic
_chemical_formula_sum            'C Cd0.8 Mg0.2 O3'
_chemical_name_mineral           Otavite
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.8670
_cell_length_b                   4.8670
_cell_length_c                   16.0787
_cell_formula_units_Z            6
_cell_volume                     329.841
_database_code_amcsd             0004326
_exptl_crystal_density_diffrn    4.676
_exptl_crystal_pressure_history  'synthesized at 600 C, 1 GPa, 3 h'
_exptl_crystal_thermal_history   'synthesized at 600 C'
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Cd.8 Mg.2) C O3'
_cod_database_code               9010205
Order and miscibility in the otavite - magnesite solid solution Sample: X_Mg = .3, synthesized at 600 C, 1 GPa, 3 h
Bromiley, F. A.; Boffa Ballaran, T.; Langenhorst, F.; Seifert, F.; American Mineralogist 92 (2007) 829–836; doi:10.2138/am.2007.2315

data_9010206
_publ_section_title
;
 Order and miscibility in the otavite - magnesite solid solution
 Sample: X_Mg = .3, synthesized at 600 C, 1 GPa, 3 h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              829
_journal_page_last               836
_journal_paper_doi               10.2138/am.2007.2315
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Synthetic
_chemical_formula_sum            'C Cd0.7 Mg0.3 O3'
_chemical_name_mineral           Otavite
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.8398
_cell_length_b                   4.8398
_cell_length_c                   15.9621
_cell_formula_units_Z            6
_cell_volume                     323.799
_database_code_amcsd             0004327
_exptl_crystal_density_diffrn    4.492
_exptl_crystal_pressure_history  'synthesized at 600 C, 1 GPa, 3 h'
_exptl_crystal_thermal_history   'synthesized at 600 C'
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Cd.7 Mg.3) C O3'
_cod_database_code               9010206
Order and miscibility in the otavite - magnesite solid solution Sample: X_Mg = .4, synthesized at 600 C, 1 GPa, 3 h
Bromiley, F. A.; Boffa Ballaran, T.; Langenhorst, F.; Seifert, F.; American Mineralogist 92 (2007) 829–836; doi:10.2138/am.2007.2315

data_9010207
_publ_section_title
;
 Order and miscibility in the otavite - magnesite solid solution
 Sample: X_Mg = .4, synthesized at 600 C, 1 GPa, 3 h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              829
_journal_page_last               836
_journal_paper_doi               10.2138/am.2007.2315
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Synthetic
_chemical_formula_sum            'C Cd0.6 Mg0.4 O3'
_chemical_name_mineral           Otavite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.8113
_cell_length_b                   4.8113
_cell_length_c                   15.8356
_cell_formula_units_Z            6
_cell_volume                     317.461
_database_code_amcsd             0004328
_exptl_crystal_density_diffrn    4.305
_exptl_crystal_pressure_history  'synthesized at 600 C, 1 GPa, 3 h'
_exptl_crystal_thermal_history   'synthesized at 600 C'
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Cd.6 Mg.4) C O3'
_cod_database_code               9010207
Order and miscibility in the otavite - magnesite solid solution Sample: X_Mg = .5, synthesized at 600 C, 1 GPa, 3 h
Bromiley, F. A.; Boffa Ballaran, T.; Langenhorst, F.; Seifert, F.; American Mineralogist 92 (2007) 829–836; doi:10.2138/am.2007.2315

data_9010208
_publ_section_title
;
 Order and miscibility in the otavite - magnesite solid solution
 Sample: X_Mg = .5, synthesized at 600 C, 1 GPa, 3 h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              829
_journal_page_last               836
_journal_paper_doi               10.2138/am.2007.2315
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Synthetic
_chemical_formula_sum            'C Cd0.5 Mg0.5 O3'
_chemical_name_mineral           Magnesite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7792
_cell_length_b                   4.7792
_cell_length_c                   15.6884
_cell_formula_units_Z            6
_cell_volume                     310.327
_database_code_amcsd             0004329
_exptl_crystal_density_diffrn    4.121
_exptl_crystal_pressure_history  'synthesized at 600 C, 1 GPa, 3 h'
_exptl_crystal_thermal_history   'synthesized at 600 C'
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Cd.5 Mg.5) C O3'
_cod_database_code               9010208
Order and miscibility in the otavite - magnesite solid solution Sample: X_Mg = .6, synthesized at 600 C, 1 GPa, 3 h
Bromiley, F. A.; Boffa Ballaran, T.; Langenhorst, F.; Seifert, F.; American Mineralogist 92 (2007) 829–836; doi:10.2138/am.2007.2315

data_9010209
_publ_section_title
;
 Order and miscibility in the otavite - magnesite solid solution
 Sample: X_Mg = .6, synthesized at 600 C, 1 GPa, 3 h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              829
_journal_page_last               836
_journal_paper_doi               10.2138/am.2007.2315
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Synthetic
_chemical_formula_sum            'C Cd0.4 Mg0.6 O3'
_chemical_name_mineral           Magnesite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7590
_cell_length_b                   4.7590
_cell_length_c                   15.5956
_cell_formula_units_Z            6
_cell_volume                     305.889
_database_code_amcsd             0004330
_exptl_crystal_density_diffrn    3.894
_exptl_crystal_pressure_history  'synthesized at 600 C, 1 GPa, 3 h'
_exptl_crystal_thermal_history   'synthesized at 600 C'
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Cd.4 Mg.6) C O3'
_cod_database_code               9010209
Order and miscibility in the otavite - magnesite solid solution Sample: X_Mg = 1, synthesized at 600 C, 1 GPa, 3 h
Bromiley, F. A.; Boffa Ballaran, T.; Langenhorst, F.; Seifert, F.; American Mineralogist 92 (2007) 829–836; doi:10.2138/am.2007.2315

data_9010210
_publ_section_title
;
 Order and miscibility in the otavite - magnesite solid solution
 Sample: X_Mg = 1, synthesized at 600 C, 1 GPa, 3 h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              829
_journal_page_last               836
_journal_paper_doi               10.2138/am.2007.2315
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Synthetic
_chemical_formula_sum            'C Mg O3'
_chemical_name_mineral           Magnesite
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.6338
_cell_length_b                   4.6338
_cell_length_c                   15.0192
_cell_formula_units_Z            6
_cell_volume                     279.288
_database_code_amcsd             0004331
_exptl_crystal_density_diffrn    3.008
_exptl_crystal_pressure_history  'synthesized at 600 C, 1 GPa, 3 h'
_exptl_crystal_thermal_history   'synthesized at 600 C'
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        'Mg C O3'
_cod_database_code               9010210
Order and miscibility in the otavite - magnesite solid solution Sample: X_Mg = .4, synthesized at 600 C, 1 GPa, 19 h
Bromiley, F. A.; Boffa Ballaran, T.; Langenhorst, F.; Seifert, F.; American Mineralogist 92 (2007) 829–836; doi:10.2138/am.2007.2315

data_9010211
_publ_section_title
;
 Order and miscibility in the otavite - magnesite solid solution
 Sample: X_Mg = .4, synthesized at 600 C, 1 GPa, 19 h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              829
_journal_page_last               836
_journal_paper_doi               10.2138/am.2007.2315
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Synthetic
_chemical_formula_sum            'C Cd0.6 Mg0.4 O3'
_chemical_name_mineral           Otavite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.8116
_cell_length_b                   4.8116
_cell_length_c                   15.8303
_cell_formula_units_Z            6
_cell_volume                     317.394
_database_code_amcsd             0004332
_exptl_crystal_density_diffrn    4.306
_exptl_crystal_pressure_history  'synthesized at 600 C, 1 GPa, 19 h'
_exptl_crystal_thermal_history   'synthesized at 600 C'
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Cd.6 Mg.4) C O3'
_cod_database_code               9010211
Order and miscibility in the otavite - magnesite solid solution Sample: X_Mg = .45, synthesized at 600 C, 1 GPa, 19 h
Bromiley, F. A.; Boffa Ballaran, T.; Langenhorst, F.; Seifert, F.; American Mineralogist 92 (2007) 829–836; doi:10.2138/am.2007.2315

data_9010212
_publ_section_title
;
 Order and miscibility in the otavite - magnesite solid solution
 Sample: X_Mg = .45, synthesized at 600 C, 1 GPa, 19 h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              829
_journal_page_last               836
_journal_paper_doi               10.2138/am.2007.2315
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Synthetic
_chemical_formula_sum            'C Cd0.55 Mg0.45 O3'
_chemical_name_mineral           Otavite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7963
_cell_length_b                   4.7963
_cell_length_c                   15.7663
_cell_formula_units_Z            6
_cell_volume                     314.104
_database_code_amcsd             0004333
_exptl_crystal_density_diffrn    4.211
_exptl_crystal_pressure_history  'synthesized at 600 C, 1 GPa, 19 h'
_exptl_crystal_thermal_history   'synthesized at 600 C'
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Cd.55 Mg.45) C O3'
_cod_database_code               9010212
Order and miscibility in the otavite - magnesite solid solution Sample: X_Mg = .5, synthesized at 600 C, 1 GPa, 19 h
Bromiley, F. A.; Boffa Ballaran, T.; Langenhorst, F.; Seifert, F.; American Mineralogist 92 (2007) 829–836; doi:10.2138/am.2007.2315

data_9010213
_publ_section_title
;
 Order and miscibility in the otavite - magnesite solid solution
 Sample: X_Mg = .5, synthesized at 600 C, 1 GPa, 19 h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              829
_journal_page_last               836
_journal_paper_doi               10.2138/am.2007.2315
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Synthetic
_chemical_formula_sum            'C Cd0.5 Mg0.5 O3'
_chemical_name_mineral           Magnesite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7813
_cell_length_b                   4.7813
_cell_length_c                   15.7023
_cell_formula_units_Z            6
_cell_volume                     310.875
_database_code_amcsd             0004334
_exptl_crystal_density_diffrn    4.114
_exptl_crystal_pressure_history  'synthesized at 600 C, 1 GPa, 19 h'
_exptl_crystal_thermal_history   'synthesized at 600 C'
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Cd.5 Mg.5) C O3'
_cod_database_code               9010213
Order and miscibility in the otavite - magnesite solid solution Sample: X_Mg = .55, synthesized at 600 C, 1 GPa, 19 h
Bromiley, F. A.; Boffa Ballaran, T.; Langenhorst, F.; Seifert, F.; American Mineralogist 92 (2007) 829–836; doi:10.2138/am.2007.2315

data_9010214
_publ_section_title
;
 Order and miscibility in the otavite - magnesite solid solution
 Sample: X_Mg = .55, synthesized at 600 C, 1 GPa, 19 h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              829
_journal_page_last               836
_journal_paper_doi               10.2138/am.2007.2315
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Synthetic
_chemical_formula_sum            'C Cd0.45 Mg0.55 O3'
_chemical_name_mineral           Magnesite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7752
_cell_length_b                   4.7752
_cell_length_c                   15.673
_cell_formula_units_Z            6
_cell_volume                     309.504
_database_code_amcsd             0004335
_exptl_crystal_density_diffrn    3.990
_exptl_crystal_pressure_history  'synthesized at 600 C, 1 GPa, 19 h'
_exptl_crystal_thermal_history   'synthesized at 600 C'
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Cd.45 Mg.55) C O3'
_cod_database_code               9010214
Order and miscibility in the otavite - magnesite solid solution Sample: X_Mg = .5, synthesized at 600 C, 1 GPa, 96 h
Bromiley, F. A.; Boffa Ballaran, T.; Langenhorst, F.; Seifert, F.; American Mineralogist 92 (2007) 829–836; doi:10.2138/am.2007.2315

data_9010215
_publ_section_title
;
 Order and miscibility in the otavite - magnesite solid solution
 Sample: X_Mg = .5, synthesized at 600 C, 1 GPa, 96 h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              829
_journal_page_last               836
_journal_paper_doi               10.2138/am.2007.2315
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Synthetic
_chemical_formula_sum            'C Cd0.5 Mg0.5 O3'
_chemical_name_mineral           Magnesite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7818
_cell_length_b                   4.7818
_cell_length_c                   15.7028
_cell_formula_units_Z            6
_cell_volume                     310.950
_database_code_amcsd             0004336
_exptl_crystal_density_diffrn    4.113
_exptl_crystal_pressure_history  'synthesized at 600 C, 1 GPa, 96 h'
_exptl_crystal_thermal_history   'synthesized at 600 C'
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Cd.5 Mg.5) C O3'
_cod_database_code               9010215
Order and miscibility in the otavite - magnesite solid solution Sample: X_Mg = .5, synthesized at 650 C, 1 GPa, 120 h
Bromiley, F. A.; Boffa Ballaran, T.; Langenhorst, F.; Seifert, F.; American Mineralogist 92 (2007) 829–836; doi:10.2138/am.2007.2315

data_9010216
_publ_section_title
;
 Order and miscibility in the otavite - magnesite solid solution
 Sample: X_Mg = .5, synthesized at 650 C, 1 GPa, 120 h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              829
_journal_page_last               836
_journal_paper_doi               10.2138/am.2007.2315
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Synthetic
_chemical_formula_sum            'C Cd0.5 Mg0.5 O3'
_chemical_name_mineral           Magnesite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7824
_cell_length_b                   4.7824
_cell_length_c                   15.7082
_cell_formula_units_Z            6
_cell_volume                     311.135
_database_code_amcsd             0004337
_exptl_crystal_density_diffrn    4.111
_exptl_crystal_pressure_history  'synthesized at 650 C, 1 GPa, 120 h'
_exptl_crystal_thermal_history   'synthesized at 650 C'
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Cd.5 Mg.5) C O3'
_cod_database_code               9010216
Order and miscibility in the otavite - magnesite solid solution Sample: X_Mg = .5, synthesized at 700 C, 1 GPa, 24 h
Bromiley, F. A.; Boffa Ballaran, T.; Langenhorst, F.; Seifert, F.; American Mineralogist 92 (2007) 829–836; doi:10.2138/am.2007.2315

data_9010217
_publ_section_title
;
 Order and miscibility in the otavite - magnesite solid solution
 Sample: X_Mg = .5, synthesized at 700 C, 1 GPa, 24 h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              829
_journal_page_last               836
_journal_paper_doi               10.2138/am.2007.2315
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Synthetic
_chemical_formula_sum            'C Cd0.5 Mg0.5 O3'
_chemical_name_mineral           Magnesite
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7820
_cell_length_b                   4.7820
_cell_length_c                   15.7028
_cell_formula_units_Z            6
_cell_volume                     310.976
_database_code_amcsd             0004338
_exptl_crystal_density_diffrn    4.113
_exptl_crystal_pressure_history  'synthesized at 700 C, 1 GPa, 24 h'
_exptl_crystal_thermal_history   'synthesized at 700 C'
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Mg.5 Cd.5) C O3'
_cod_database_code               9010217
Order and miscibility in the otavite - magnesite solid solution Sample: X_Mg = 0, synthesized at 800 C, 1 GPa, 1 h
Bromiley, F. A.; Boffa Ballaran, T.; Langenhorst, F.; Seifert, F.; American Mineralogist 92 (2007) 829–836; doi:10.2138/am.2007.2315

data_9010218
_publ_section_title
;
 Order and miscibility in the otavite - magnesite solid solution
 Sample: X_Mg = 0, synthesized at 800 C, 1 GPa, 1 h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              829
_journal_page_last               836
_journal_paper_doi               10.2138/am.2007.2315
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Synthetic
_chemical_formula_sum            'C Cd O3'
_chemical_name_mineral           Otavite
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.9204
_cell_length_b                   4.9204
_cell_length_c                   16.2948
_cell_formula_units_Z            6
_cell_volume                     341.649
_database_code_amcsd             0004339
_exptl_crystal_density_diffrn    5.028
_exptl_crystal_pressure_history  'synthesized at 800 C, 1 GPa, 1 h'
_exptl_crystal_thermal_history   'synthesized at 800 C'
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        'Cd C O3'
_cod_database_code               9010218
Order and miscibility in the otavite - magnesite solid solution Sample: X_Mg = .1, synthesized at 800 C, 1 GPa, 1 h
Bromiley, F. A.; Boffa Ballaran, T.; Langenhorst, F.; Seifert, F.; American Mineralogist 92 (2007) 829–836; doi:10.2138/am.2007.2315

data_9010219
_publ_section_title
;
 Order and miscibility in the otavite - magnesite solid solution
 Sample: X_Mg = .1, synthesized at 800 C, 1 GPa, 1 h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              829
_journal_page_last               836
_journal_paper_doi               10.2138/am.2007.2315
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Synthetic
_chemical_formula_sum            'C Cd0.9 Mg0.1 O3'
_chemical_name_mineral           Otavite
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.8934
_cell_length_b                   4.8934
_cell_length_c                   16.1892
_cell_formula_units_Z            6
_cell_volume                     335.720
_database_code_amcsd             0004340
_exptl_crystal_density_diffrn    4.855
_exptl_crystal_pressure_history  'synthesized at 800 C, 1 GPa, 1 h'
_exptl_crystal_thermal_history   'synthesized at 800 C'
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Cd.9 Mg.1) C O3'
_cod_database_code               9010219